Aqueous Synthesis of Ru Doped Hematite Nanostructures: A Morphological, Structural, Optical, and Magnetic Study

1Department of Physics and Engineering, University of Zululand, Private Bag X1001, Kwadlangezwa 3886, South Africa 2Nanosciences African Network (NANOAFNET), iThemba LABS, National Research Foundation, P.O. Box 722, Somerset West, Western Cape 7129, South Africa 3Physics Department, Durban University of Technology, Durban 4001, South Africa 4UNESCO-UNISA Africa Chair in Nanosciences and Nanotechnology, College of Graduate Studies, University of South Africa, Muckleneuk Ridge, P.O. Box 392, Pretoria 0002, South Africa


Introduction
Hematite (-Fe 2 O 3 ) is the thermodynamically stable crystallographic phase of ferric oxide.It is earth abundant, nontoxic, and photocorrosive resistant and is an efficient photocatalytic material [1].Because of the bulk band gap of 1.9-2.2eV, hematite was recognized as an ideal candidate as photoanode material in a Photoelectrochemical Cell (PEC) for the production of hydrogen by solar water splitting process.
Thin films of hematite, consisting of crystalline arrays of oriented nanorods [2], have been demonstrated to display efficient photovoltaic properties [2].In view of the relatively large charge carrier free mean path and e-hole recombination, these oriented nanorods provide better transport and collection of photogenerated electrons, exhibiting substantial photocurrent efficiency.A higher level of engineering of -Fe 2 O 3 based nanomaterials, such as 3-dimensional and anisotropic oriented arrays, is currently under investigation for additional potential technological applications in electronics, photonics, and magnetic devices.Current methods of preparation of such nanorods involve various approaches, such as chemical vapour deposition [3], sol-gel processes [4], pulsed laser evaporation [5], reactive sputtering [6], hydrothermal techniques [7], spray pyrolysis [8], and aqueous chemical growth (ACG) [9].In the present study, ACG, also known as Vayssieres method, was adopted to grow hematite nanorods, because it is a simple technique for nanostructure deposition at relatively low temperatures.Advantages of the ACG method include the utilization of nonexpensive equipment, nontoxic reagents, nonhazardous byproducts, and surfactant-free surfaces.The morphology, shape, size, and structure of grown nanostructures can be tailored by adjusting growth parameters, such as the concentration of the solution, the reagent stoichiometry, the temperature, and the pH [10].The present study focusses on the effects of Ru doping on the optical, morphological, and structural properties of hematite nanorods.fluorine doped tin oxide (FTO) glass substrates using the ACG method.The commercially high grade chemicals (purchased from Industrial Analytical Ltd.) used in the synthesis were ferric chloride (FeCl 3 ), sodium nitrate (NaNO 3 ), and ruthenium chloride (RuCl 3 ⋅xH 2 O).The precursor concentrations used in the synthesis were 0.1 Molar of anhydrous FeCl 3 and 1 Molar of NaNO 3 .The deposition temperature was set at 95 ∘ C. FTO substrates cut to the required dimensions (25 × 25 mm 2 ) were cleaned by ultrasonic washing and degreased with trichloroethylene, acetone, and methanol consecutively.The clean substrates were immersed into 100 mL aqueous solution (MilliQ, 18.2 MΩ cm) of FeCl 3 and NaNO 3 (pH of 1.5) and placed in a standard laboratory oven at a constant temperature of 95 ∘ C for different deposition times.The pH of 1.5 allows the growth of perpendicularly oriented nanorods with the longest length and the smallest diameter [12,13].The resultant thin films were thoroughly washed with deionized water to remove any residual salts and then dried at 95 ∘ C for 1 h.The thin films were heat treated in air at 500 ∘ C for 1 h to obtain the desired stoichiometric and thermodynamically stable hematite phase of -Fe 2 O 3 .

Material Characterization.
The crystallinity of the deposited iron oxide thin films was characterized by X-ray diffraction (XRD), using a Bruker AXS D8 Advance X-ray diffractometer with Cu K radiation ( = 1.541Å).The XRD data were collected with a position sensitive detector (PSD) at scan steps of 0.007 ∘ and scan speed of 1 step/s.The morphology of the films was studied using a Leo-Stereo Scan 440 Scanning Electron Microscope (SEM), while the chemical composition and physical properties of the -Fe 2 O 3 particles were investigated using Raman spectroscopy and Mössbauer spectroscopy.The Mössbauer spectra of the samples were collected in transmission mode using a 15 mCi 57 CoRh source.UV-VIS-NIR optical measurements, both direct transmission () and absorption (), were carried out within the spectral range of 200-1100 nm, at room temperature on a Cecil 2000 spectrophotometer.Wavenumber (cm −1 ) are due to reflections from the glass substrate.The atomic concentrations of Ru in the samples were estimated to be 0.14, 0.08, and 0.06 at.% for the samples synthesized with 0.030 g, 0.018 g, and 0.006 g of RuCl 3 ⋅xH 2 O precursor, respectively.

Results and Discussion
Figure 4 reports the SEM images of the undoped and the various Ru doped hematite samples.All samples exhibit the expected morphology and shape anisotropy of the synthesized particles: nanorods.Likewise, it can be noted that the higher the doping is, the more random the orientation of the nanorods is.Yet this misorientation is effective; it would not a priori affect the carrier charge free mean path but would enhance the light trapping due to multiple scattering.Consequentially, the overall water photosplitting efficiency would be high accordingly.

Raman Analysis on Ru Doped Hematite Nanorods.
The Raman spectra for Ru doped hematite samples are shown in Figure 5.All vibrational modes for hematite are present, as summarized in Table 1.The intensity of the E g (1) vibrational mode, positioned at 288 cm −1 , decreases with increasing dopant concentration.The vibrational mode around 1124 cm −1 is due to Ru-O bonds as reported by Jo et al. (2005) [11].The higher the dopant concentration, the lesser the intensity and the broader the width of the vibration modes.This indicates the loss of crystallinity in the samples when the dopant concentrations increase at least locally.This could be correlated to the broadening of the XRD patterns as reported above.

Analysis of Mössbauer Spectra.
Mössbauer spectra of the unheated and heated Ru doped samples are presented in Figures 6 and 7, respectively.The spectra were analysed with the analysis code RECOIL [14], using Lorentzian line shapes.The hyperfine parameters extracted from the fits to  the spectra are presented in Table 2, in which the isomer shifts are expressed relative to -Fe.The spectra of the as-synthesized samples consist of doublets whose isomer shifts and quadrupole splittings are close to those of -Fe 2 O 3 [15].However, in the case -Fe 2 O 3 the two subspectra have quadrupole shifts of 0.69 and 0.90 mm/s, which are quite different from the values extracted from our fits to the spectrum obtained for the sample synthesized with 0.030 g of the Ru precursor (Figure 6(c)).This leads us to conclude that the synthesized thin films consist of nanoclusters of -Fe 2 O 3 which display superparamagnetic relaxation in their RT spectra.On annealing at 500 ∘ C, the nanoclusters morph into nanorods, as shown in Figure 4.The Mössbauer spectra evolve into magnetic sextets expected of multidomain structures.The spectra show some very interesting features.In the case of the 0.018 g doped sample, in addition to the main sextet with a hyperfine field close to that of -Fe 2 O 3 , the spectra also show approximately 30% contribution from components with lower field values with large line widths, presumably due to amorphous Fe(III) complexes.The main sextet consists of two subspectra.This is more clearly visible in the spectrum of the sample synthesized with 0.030 g of the precursor (Figure 7(d)).In addition to the sextet with a magnetic hyperfine field of  = 5.12 T, a new sextet with  = 5.26 T is required to fit the data.This feature is very similar to that displayed in Figure 2 of [14], of pure synthetic hematite at 260 K (i.e., at the Morin temperature) showing the coexistence of the antiferromagnetic and weakly ferromagnetic phases.Our MS results, obtained in RT measurements, show that the Ru dopant raises the Morin temperature of hematite, in agreement with the observations reported by Helgason et al. [16], and provides further evidence that the Ru ions are incorporated in the -Fe 2 O 3 structure.

Optical Properties of Ru Doped Hematite Nanorods.
Figure 8 presents the UV-VIS-NIR optical transmissions of Ru doped hematite thin film samples.The transmission decreases as the dopant increases; such a trend could be correlated with the higher orientation disorder induced by the Ru doping as observed previously in the SEM imaging.The corresponding optical absorbance spectra are presented in Figure 9.The latter were used to derive the optical band gap of the samples.It has been reported that the band edge position can be tailored by the electronegativity of the dopants as well as by quantum confinement effects.Figure 10 presents the plot of the (ℎ]) 2 as a function of ℎ] from which the optical band gap of the Ru dope hematite nanorods was estimated to be 2.32 eV and 2.36 eV for the samples deposited with 0.006 g and 0.018 g of the precursor and for the sample prepared with 0.030 g of RuCl 3 ⋅xH 2 O it was found to be 2.48 eV.This indicates a shift within the range of 0.26-0.56eV for both samples prepared with 0.006 and 0.018 g of RuCl 3 ⋅xH 2 O doping precursor and 0.29-0.59eV for sample deposited with 0.030 g of RuCl 3 ⋅xH 2 O doping precursor.These shifts are in line with the targeted blue shift of the hematite band gap of about 0.3 to 0.6 eV [12] which induce the upward shift of the conduction band edge.This substantial increase in the optical band gap could be due to a combination of the dopant as well as quantum confinement effects.It has been reported that the optimal band gap of 2.46 eV [12,13] is required for water photooxidation without an external bias.Therefore, our obtained values would allow engineering a water splitting device without external bias.

Conclusion
The controlled growth of uniform Ru--Fe 2 O 3 nanorods at a low temperature with soft chemistry deposition technique (ACG) was achieved.The XRD peak pattern broadening and the peak position shifts, because of increased dopant  Zululand, South Africa, and the National Research Foundation (South Africa).

Figure 2 :
Figure 2: Average basal size of the grown nanorods as a function of doping, estimated from the width of the (104) Bragg peak.

Figure 6 :
Figure 6: Mössbauer spectra of the as-synthesized (unheated) Ru doped iron oxide powder samples deposited for 24 h, using the precursor concentrations shown.

Figure 10 :
Figure10: The band gap estimation deduced from plots of (ℎ]) 2 as a function of photon energy (ℎ]) for Ru doped hematite thin films grown on FTO glass substrate at 95 ∘ C for 24 h, where A is undoped, B is 0.006 g, C is 0.018 g, and D is 0.03 g of RuCl 3 ⋅xH 2 O.
Figure 1 reports the 2 XRD scans of the hematite nanostructures for the various Ru doping concentrations.According to the JCPDC database, number 73-0603 and number 1309-37-1 of -Fe 2 O 3, the peaks corresponding to the values of 2 equal to 24.14 ∘ , 33.15 ∘ , 35.61 ∘ , 39.28 ∘ , 40.86 ∘ , 49.48 ∘ , 54.09 ∘ , 56.15 ∘ , 57.59 ∘ , 62.45 ∘ , and 63.99 ∘ 3.1.Crystallographic Structure and X-Rays Diffraction.respectively.The intensity of the component along the (104) plane indicates that the Ru doped hematite particles are oriented in {104} direction.The intensity of this strongest peak tends to decrease and its line width broadens as the Ru dopant concentration increases.More precisely, the (104) Bragg peak becomes less intense than the (110) and hence

Table 1 :
The Raman shifts (cm −1 ) for the Ru doped hematite nanorods grown for 24 h on FTO glass substrate, where A presents data for pure Fe 2 O 3 , B for 0.006 g, C for 0.018 g, and D for 0.030 g precursor doped samples.

Table 2 :
Mössbauer parameters (isomer shift (CS), quadrupole splitting (QS), hyperfine field (H), line width (HWHM), and area fraction (A)) extracted from the fits to the spectra displayed in Figures6 and 7, of the Ru doped -Fe 2 O 3 samples synthesized with the precursor concentrations shown.The isomer shifts are expressed relative to -Fe.